MIL-HDBK-5H, Change Notice 11 October 20011-1Supersedes Chapter 1 of Revision HCHAPTER 1GENERAL1.1 PURPOSE AND USE OF DOCUMENT1.1.1 INTRODUCTION — Since many aerospace companies manufacture both commercial andmilitary products, the standardization of metallic materials design data, which are acceptable to Governmentprocuring or certification agencies is very beneficial to those manufacturers as well as governmental agencies.Although the design requirements for militaryand commercial products maydiffer greatly, the required designvalues for the strength of materials and elements and other needed material characteristics are often identical.Therefore, this publication provides standardized design values and related design information for metallicmaterials and structural elements used in aerospace structures. The data contained herein, or from approveditems in the minutes of MIL-HDBK-5 coordination meetings, are acceptable to the Air Force, the Navy, theArmy, and the Federal Aviation Administration. Approval by the procuring or certificating agency must beobtained for the use of design values for products not contained herein.This printed document is distributed by the Defense Area Printing Service (DAPS). It is the onlyofficialformofMIL-HDBK-5. IfcomputerizedMIL-HDBK-5databasesareused,cautionshouldbeexercisedto ensure that the information in these databases is identical to that contained in this Handbook.U.S.Government personnel mayobtain free copies of the current version of the printed document fromthe Defense Area Printing Service (DAPS). Assistance with orders may be obtained by calling (215) 697-2179. The FAX number is (215) 697-1462. Alternatively, DD Form 1425, as enclosed on page 1-37, may befilled out and mailed to:DODSSP700 Robbins Avenue, Building 4DPhiladelphia, PA 19111-5094U.S. Government personnel may also obtain a free electronic copy of the current document fromDAPS through the ASSIST website at http://assist.daps.mil.As noted on the front page, the current version of MIL-HDBK-5 is copyrighted. No part of thisdocument may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means,electronic, mechanical,photocopying, recording, or otherwise, without the written permission of the copyrightowner.1.1.2 SCOPE OF HANDBOOK — This Handbook is primarily intended to provide a source of designmechanical and physical properties, and joint allowables. Material property and joint data obtained from testsby material and fastener producers, government agencies, and members of the airframe industry are submittedto MIL-HDBK-5 for review and analysis. Results of these analyses are submitted to the membership duringsemi-annual coordination meetings for approval and, when approved, published in this Handbook.This Handbook also contains some useful basic formulas for structural element analysis. However,structural design and analysis are beyond the scope of this Handbook.
MIL-HDBK-5H, Change Notice 11 October 20011-2Supersedes Chapter 1 of Revision HReferences for data and various test methods are listed at the end of each chapter. The referencenumber corresponds to the applicable paragraph of the chapter cited. Such references are intended to providesources of additional information, but should not necessarily be considered as containing data suitable fordesign purposes.The content of this Handbook is arranged as follows:Chapter(s) Subjects1 Nomenclature, Systems of Units, Formulas, Material Property Definitions,Failure Analysis, Column Analysis, Thin-Walled Sections2-7 Material Properties8 Joint Allowables9 Data Requirements, Statistical Analysis Procedures1.2 NOMENCLATURE1.2.1 SYMBOLS AND DEFINITIONS — The various symbols used throughout the Handbook todescribe properties of materials, grain directions, test conditions, dimensions, and statistical analysisterminology are included in Appendix A.1.2.2 INTERNATIONAL SYSTEM OF UNITS (SI) — Design properties and joint allowablescontained in this Handbook are given in customary units of U.S. measure to ensure compatibility withgovernment and industry material specifications and current aerospace design practice. Appendix A.4 maybe used to assist in the conversion of these units to Standard International (SI) units when desired.1.3 COMMONLY USED FORMULAS1.3.1 GENERAL — Formulas provided in the following sections are listed for referencepurposes. Sign conventions generally accepted in their use are that quantities associated with tension action(loads, stresses, strains, etc., are usually considered as positive and quantities associated with compressiveaction are considered as negative. When compressive action is of primary interest, it is sometimes convenientto identify associated properties with a positive sign. Formulas for all statistical computations relating toallowables development are presented in Chapter 220.127.116.11 SIMPLE UNIT STRESSES —ft = P / A (tension) [1.3.2(a)]fc = P / A (compression) [1.3.2(b)]fb = My / I = M / Z [1.3.2(c)]fs = S / A (average direct shear stress) [1.3.2(d)]fx = SQ / Ib (longitudinal or transverse shear stress) [1.3.2(e)]fx = Ty / Ip (shear stress in round tubes due to torsion) [1.3.2(f)]fs = (T/2At) (shear stress due to torsion in thin-walled structures of closed section. Note [1.3.2(g)]that A is the area enclosed by the median line of the section.)fA = BfH ; fT = BfL [1.3.2(h)]
MIL-HDBK-5H, Change Notice 11 October 20011-3Supersedes Chapter 1 of Revision H1.3.3 COMBINED STRESSES (SEE SECTION 18.104.22.168) —fA = fc + fb (compression and bending) [1.3.3(a)](compression, bending, and torsion) [1.3.3(b)]( )[ ]f f fs s nmax//= +2 2 1 22fn max = fn/2 + fs max [1.3.3(c)]1.3.4 DEFLECTIONS (AXIAL) —e = δ / L (unit deformation or strain) [1.3.4(a)]E = f/e (This equation applied when E is obtained from the same tests in which [1.3.4(b)]f and e are measured.)δ = eL = (f / E)L [1.3.4(c)]= PL / (AE) (This equation applies when the deflection is to be [1.3.4(d)]calculated using a known value of E.)1.3.5 DEFLECTIONS (BENDING) —di/dx = M / (EI) (Change of slope per unit length of a beam; radians per unit length) [1.3.5(a)]— Slope at Point 2. (This integral denotes the area under the 1.3.5(b)][ ]i i M EI dxxx2 112= + ∫ /( )curve of M/EI plotted against x, between the limits of x1 and x2.)— Deflection at Point 2. [1.3.5(c)]( ) ( )( )y y i x x M EI x x dxxx2 1 2 1 212= + − + −∫ /(This integral denotes the area under the curve having an ordinate equal to M/EI multiplied by thecorresponding distances to Point 2, plotted against x, between the limits of x1 and x2.)— Deflection at Point 2. (This integral denotes the area under the [1.3.5(d)]y y idxxx2 112= + ∫ curve of x1(i) plotted against x, between the limits of x1 and x2.)1.3.6 DEFLECTIONS (TORSION) —dφ / dx = / T / (GJ) (Change of angular deflection or twist per unit length of a member, [1.3.6(a)]radians per unit length.)— Total twist over a length from x1 to x2. (This integral denotes the [1.3.6(b)][ ]Φ = ∫ T GJ dxxx/ ( )12area under the curve of T/GJ plotted against x, between the limitsof x1 and x2.)Φ = TL/(GJ) (Used when torque T/GJ is constant over length L.) [1.3.6(c)]
MIL-HDBK-5H, Change Notice 11 October 20011-4Supersedes Chapter 1 of Revision H1.3.7 BIAXIAL ELASTIC DEFORMATION —µ = eT/eL (Unit lateral deformation/unit axial deformation.) This identifies Poisson’s ratio [1.3.7(a)]in uniaxial loading.Eex = fx - µfy [1.3.7(b)]Eey = fy - µfx [1.3.7(c)]Ebiaxial = E(1 - µB) — B = biaxial elastic modulus. [1.3.7(d)]1.3.8 BASIC COLUMN FORMULAS —Fc = π2Et (LN / ρ)2where LN = L / %&c — conservative using tangent modulus [1.3.8(a)]Fc = π2E (LN / ρ)2— standard Euler formula [1.3.8(b)]1.4 BASIC PRINCIPLES1.4.1 GENERAL — It is assumed that users of this Handbook are familiar with the principles ofstrength of materials. A brief summary of that subject is presented in the following paragraphs to emphasizeprinciples of importance regarding the use of allowables for various metallic materials.Requirements for adequate test data have been established to ensure a high degree of reliability forallowables published in this Handbook. Statistical analysis methods, provided in Chapter 9, are standardizedand approved by all government regulatory agencies as well as MIL-HDBK-5 members from industry.22.214.171.124 Basis — Primary static design properties are provided for the following conditions:Tension . . . . . . . . . Ftu and FtyCompression . . . . . FcyShear . . . . . . . . . . . FsuBearing . . . . . . . . . . Fbru and FbryThese design properties are presented as A- and B- or S-basis room temperature values for each alloy. Designproperties for other temperatures, when determined in accordance with Section 126.96.36.199, are regarded as havingthe same basis as the corresponding room temperature values.Elongationandreductionofareadesignpropertieslistedinroomtemperaturepropertytablesrepresentprocurement specification minimum requirements, and are designated as S-values. Elongation and reductionof area at other temperatures, as well as moduli, physical properties, creep properties, fatigue properties andfracture toughness properties are all typical values unless another basis is specifically indicated.Use of B-Values — The use of B-basis design properties is permitted in design by the Air Force, theArmy, the Navy, and the Federal Aviation Administration, subject to certain limitations specified by eachagency. Reference should be made to specific requirements of the applicable agency before using B-valuesin design.
MIL-HDBK-5H, Change Notice 11 October 20011-5Supersedes Chapter 1 of Revision H188.8.131.52 Statistically Calculated Values — Statistically calculated values are S (since 1975),T99 and T90. S, the minimum properties guaranteed in the material specification, are calculated using the samerequirements and procedure as AMS and is explained in Chapter 9. T99 and T90 are the local tolerance bounds,and are defined and may be computed using the data requirements and statistical procedures explained inChapter 184.108.40.206.3 Ratioed Values — A ratioed design property is one that is determined through itsrelationship with an established design value. This may be a tensile stress in a different grain direction fromthe established design property grain direction, or it may be another stress property, e.g., compression, shearor bearing. It may also be the same stress property at a different temperature. Refer to Chapter 9 for specificdata requirements and data analysis procedures.Derived properties are presented in two manners. Room temperature derived properties are presentedin tabular form with their baseline design properties. Other than room temperature derived properties arepresented in graphical form as percentages of the room temperature value. Percentage values apply to allforms and thicknesses shown in the room temperature design property table for the heat treatment conditionindicated therein unless restrictions are otherwise indicated. Percentage curves usually represent short timeexposures to temperature (thirty minutes) followed by testing at the same strain rate as used for the roomtemperature tests. When data are adequate, percentage curves are shown for other exposure times and areappropriately labeled.1.4.2 STRESS — The term “stress” as used in this Handbook implies a force per unit area and is ameasure of the intensity of the force acting on a definite plane passing through a given point (see Equations1.3.2(a) and 1.3.2(b)). The stress distribution may or may not be uniform, depending on the nature of theloading condition. For example, tensile stresses identified by Equation 1.3.2(a) are considered to be uniform.The bending stress determined from Equation 1.3.2(c) refers to the stress at a specified distance perpendicularto the normal axis. The shear stress acting over the cross section of a member subjected to bending is notuniform. (Equation 1.3.2(d) gives the average shear stress.)1.4.3 STRAIN — Strain is the change in length per unit length in a member or portion of a member.As in the case of stress, the strain distribution may or may not be uniform in a complex structural element,depending on the nature of the loading condition. Strains usually are present also in directions other that thedirections of applied loads.220.127.116.11 Poisson’s Ratio Effect — A normal strain is that which is associated with a normalstress; a normal strain occurs in the direction in which its associated normal stress acts. Normal strains thatresult from an increase in length are designated as positive (+) and those that result in a decrease in length aredesignated as negative (-).Under the condition of uniaxial loading, strain varies directly with stress. The ratio of stress to strainhas a constant value (E) within the elastic range of the material, but decreases when the proportional limit isexceeded (plastic range). Axial strain is always accompanied by lateral strains of opposite sign in the twodirections mutually perpendicular to the axial strain. Under these conditions, the absolute value of a ratio oflateral strain to axial strain is defined as Poisson’s ratio. For stresses within the elastic range, this ratio isapproximately constant. For stresses exceeding the proportional limit, this ratio is a function of the axial strainand is then referred to as the lateral contraction ratio. Information on the variation of Poisson’s ratio withstrain and with testing direction is available in Reference 18.104.22.168.Under multiaxial loading conditions, strains resulting fromthe application of each directional load areadditive. Strains must be calculated for each of the principal directions taking into account each of theprincipal stresses and Poisson’s ratio (see Equations 22.214.171.124 and 126.96.36.199 for biaxial loading).
MIL-HDBK-5H, Change Notice 11 October 20011-6Supersedes Chapter 1 of Revision H188.8.131.52 Shear Strain — When an element of uniform thickness is subjected to pure shear, eachside of the element will be displaced in opposite directions. Shear strain is computed by dividing this totaldisplacement by the right angle distance separating the two sides.184.108.40.206 Strain Rate — Strain rate is a function of loading rate. Test results are dependent uponstrain rate, and the ASTM testing procedures specify appropriate strain rates. Design properties in thisHandbook were developed from test data obtained from coupons tested at the stated strain rate or up to a valueof 0.01 in./in./min, the standard maximum static rate for tensile testing materials per specification ASTM E220.127.116.11.4 Elongation and Reduction of Area — Elongation and reduction of area are measuredin accordance with specification ASTM E 18.104.22.168 TENSILE PROPERTIES — When a metallic specimen is tested in tension using standardprocedures of ASTM E 8, it is customary to plot results as a “stress-strain diagram.” Typical tensile stress-strain diagrams are characterized in Figure 1.4.4. Such diagrams, drawn to scale, are provided in appropriatechapters of this Handbook. The general format of such diagrams is to provide a strain scale nondimensionally(in./in.) and a stress scale in 1000 lb/in. (ksi). Properties required for design and structural analysis arediscussed in Sections 22.214.171.124 to 126.96.36.199.188.8.131.52 Modulus of Elasticity (E) — Referring to Figure 1.4.4, it is noted that the initial part ofstress-strain curves are straight lines. This indicates a constant ratio between stress and strain. Numericalvalues of such ratios are defined as the modulus of elasticity, and denoted by the letter E. This value appliesup to the proportional limit stress at which point the initial slope of the stress-strain curve then decreases.Modulus of elasticity has the same units as stress. See Equation 1.3.4 (b).Other moduli of design importance are tangent modulus, Et, and secant modulus, Es. Both of thesemoduli are functions of strain. Tangent modulus is the instantaneous slope of the stress-strain curve at anyselected value of strain. Secant modulus is defined as the ratio of total stress to total strain at any selectedvalue of strain. Both of these moduli are used in structural element designs. Except for materials such as thosedescribed with discontinuous behaviors, such as the upper stress-strain curve in Figure 1.4.4, tangent modulusis the lowest value of modulus at any state of strain beyond the proportional limit. Similarly, secant modulusis the highest value of modulus beyond the proportional limit.Clad aluminum alloys may have two separate modulus of elasticity values, as indicated in the typicalstress-strain curve shown in Figure 1.4.4. The initial slope, or primary modulus, denotes a response of boththe low-strength cladding and higher-strength core elastic behaviors. This value applies only up to theproportional limit of the cladding. For example, the primary modulus of 2024-T3 clad sheet applies only upto about 6 ksi. Similarly, the primary modulus of 7075-T6 clad sheet applies only up to approximately 12 ksi.A typical use of primary moduli is for low amplitude, high frequency fatigue. Primary moduli are notapplicable at higher stress levels. Above the proportional limits of cladding materials, a short transition rangeoccurs while the cladding is developing plastic behavior. The material then exhibits a secondary elasticmodulus up to the proportional limit of the core material. This secondary modulus is the slope of the secondstraight line portion of the stress-strain curve. In some cases, the cladding is so little different from the corematerial that a single elastic modulus value is used.
MIL-HDBK-5H, Change Notice 11 October 20011-7Supersedes Chapter 1 of Revision HFigure 1.4.4. Typical tensile stress-strain diagrams.
MIL-HDBK-5H, Change Notice 11 October 20011-8Supersedes Chapter 1 of Revision H184.108.40.206 Tensile Proportional Limit Stress (Ftp) — The tensile proportional limit is themaximum stress for which strain remains proportional to stress. Since it is practically impossible to determineprecisely this point on a stress-strain curve, it is customary to assign a small value of plastic strain to identifythe corresponding stress as the proportional limit. In this Handbook, the tension and compression proportionallimit stress corresponds to a plastic strain of 0.0001 in./in.220.127.116.11 Tensile Yield Stress (TYS or Fty) — Stress-strain diagrams for some ferrous alloysexhibit a sharp break at a stress below the tensile ultimate strength. At this critical stress, the materialelongates considerably with no apparent change in stress. See the upper stress-strain curve in Figure 1.4.4.The stress at which this occurs is referred to as the yield point. Most nonferrous metallic alloys and most highstrength steels do not exhibit this sharp break, but yield in a monotonic manner. This condition is alsoillustrated in Figure 1.4.4. Permanent deformation may be detrimental, and the industry adopted 0.002 in./in.plastic strain as an arbitrary limit that is considered acceptable by all regulatory agencies. For tension andcompression, the corresponding stress at this offset strain is defined as the yield stress (see Figure 1.4.4). Thisvalue of plastic axial strain is 0.002 in./in. and the corresponding stress is defined as the yield stress. Forpractical purposes, yield stress can be determined from a stress-strain diagram by extending a line parallel tothe elastic modulus line and offset from the origin by an amount of 0.002 in./in. strain. The yield stress isdetermined as the intersection of the offset line with the stress-strain curve.18.104.22.168 Tensile Ultimate Stress (TUS or Fty) — Figure 1.4.4 shows how the tensile ultimatestress is determined from a stress-strain diagram. It is simply the maximum stress attained. It should be notedthat all stresses are based on the original cross-sectional dimensions of a test specimen, without regard to thelateral contraction due to Poisson’s ratio effects. That is, all strains used herein are termed engineering strainsas opposed to true strains which take into account actual cross sectional dimensions. Ultimate tensile stressis commonly used as a criterion of the strength of the material for structural design, but it should be recognizedthat other strength properties may often be more important.22.214.171.124 Elongation (e) — An additional property that is determined from tensile tests iselongation. This is a measure of ductility. Elongation, also stated as total elongation, is defined as thepermanent increase in gage length, measured after fracture of a tensile specimen. It is commonly expressedas a percentage of the original gage length. Elongation is usually measured over a gage length of 2 inches forrectangular tensile test specimens and in 4D (inches) for round test specimens. Welded test specimens areexceptions. Refer to the applicable material specification for applicable specified gage lengths. Althoughelongation is widely used as an indicator of ductility, this property can be significantly affected by testingvariables, such as thickness, strain rate, and gage length of test specimens. See Section 126.96.36.199 for data basis.188.8.131.52 Reduction of Area (RA) — Another property determined from tensile tests is reductionof area, which is also a measure of ductility. Reduction of area is the difference, expressed as a percentage ofthe original cross sectional area, between the original cross section and the minimum cross sectional areaadjacent to the fracture zone of a tested specimen. This property is less affected by testing variables thanelongation, but is more difficult to compute on thin section test specimens. See Section 184.108.40.206 for data basis.1.4.5 COMPRESSIVE PROPERTIES — Results of compression tests completed in accordance withASTM E 9 are plotted as stress-strain curves similar to those shown for tension in Figure 1.4.4. Precedingremarks concerning tensile properties of materials, except for ultimate stress and elongation, also apply tocompressive properties. Moduli are slightly greater in compression for most of the commonly used structuralmetallic alloys. Special considerations concerning the ultimate compressive stress are described in thefollowing section. An evaluation of techniques for obtaining compressive strength properties of thin sheetmaterials is outlined in Reference 1.4.5.
MIL-HDBK-5H, Change Notice 11 October 20011-9Supersedes Chapter 1 of Revision H220.127.116.11 Compressive Ultimate Stress (Fcu) – Since the actual failure mode for the highesttension and compression stress is shear, the maximum compression stress is limited to Ftu. The driver for allthe analysis of all structure loaded in compression is the slope of the compression stress strain curve, thetangent modulus.18.104.22.168 Compressive Yield Stress (CYS or Fcy) — Compressive yield stress is measured in amanner identical to that done for tensile yield strength. It is defined as the stress corresponding to 0.002 in./in.plastic strain.1.4.6 SHEAR PROPERTIES — Results of torsion tests on round tubes or round solid sections areplotted as torsion stress-strain diagrams. The shear modulus of elasticity is considered a basic shear property.Other properties, such as the proportional limit stress and shear ultimate stress, cannot be treated as basic shearproperties because of “form factor” effects. The theoretical ratio between shear and tensile stress forhomogeneous, isotropic materials is 0.577. Reference 1.4.6 contains additional information on this subject.22.214.171.124 Modulus of Rigidity (G) — This property is the initial slope of the shear stress-straincurve. It is also referred to as the modulus of elasticity in shear. The relation between this property and themodulus of elasticity in tension is expressed for homogeneous isotropic materials by the following equation:[126.96.36.199]GE=+2 1( )µ188.8.131.52 Proportional Limit Stress in Shear (Fsp) — This property is of particular interest inconnection with formulas which are based on considerations of linear elasticity, as it represents the limitingvalue of shear stress for which such formulas are applicable. This property cannot be determined directly fromtorsion tests.184.108.40.206 Yield and Ultimate Stresses in Shear (SYS or Fsy) and (SUS or Fsu) — Theseproperties, as usually obtained from ASTM test procedures tests, are not strictly basic properties, as they willdepend on the shape of the test specimen. In such cases, they should be treated as moduli and should not becombined with the same properties obtained from other specimen configuration tests.Design values reported for shear ultimate stress (Fsu) in roomtemperature propertytables for aluminumand magnesium thin sheet alloys are based on “punch” shear type tests except when noted. Heavy section testdata are based on “pin” tests. Thin aluminum products may be tested to ASTM B 831, which is a slotted sheartest (this test is used for other alloys; however, the standard doesn’t specifically cover materials other thanaluminum). Thicker aluminums use ASTM B 769, otherwise known as the Amsler shear test. These two testsonly provide ultimate strength. Shear data for other alloys are obtained from pin tests, except where productthicknesses are insufficient.1.4.7 BEARING PROPERTIES — Bearing stress limits are of value in the design of mechanicallyfastened joints and lugs. Only yield and ultimate stresses are obtained from bearing tests. Bearing stress iscomputed from test data by dividing the load applied to the pin, which bears against the edge of the hole, bythe bearing area. Bearing area is the product of the pin diameter and the sheet or plate thickness.A bearing test requires the use of special cleaning procedures as specified in ASTM E 238. Resultsare identified as “dry-pin” values. The same tests performed without application of ASTM E 238 cleaningprocedures are referred to as “wet pin” tests. Results from such tests can show bearing stresses at least 10percent lower than those obtained from “dry pin” tests. See Reference 1.4.7 for additional information.
MIL-HDBK-5H, Change Notice 11 October 20011-10Supersedes Chapter 1 of Revision HAdditionally, ASTM E 238 requires the use of hardened pins that have diameters within 0.001 of the holediameter. As the clearance increases to 0.001 and greater, the bearing yield and failure stress tends to decrease.In the definition of bearing values, t is sheet or plate thickness, D is the pin diameter, and e is the edgedistance measured from the center of the hole to the adjacent edge of the material being tested in the directionof applied load.220.127.116.11 Bearing Yield and Ultimate Stresses (BYS or Fbry) and (BUS or Fbru) — BUS isthe maximum stress withstood by a bearing specimen. BYS is computed from a bearing stress-deformationcurve by drawing a line parallel to the initial slope at an offset of 0.02 times the pin diameter.Tabulated design properties for bearingyield stress(Fbry) and bearingultimate stress (Fbru) are providedthroughout the Handbook for edge margins of e/D = 1.5 and 2.0. Bearing values for e/D of 1.5 are not intendedfor designs of e/D < 1.5. Bearing values for e/D < 1.5 must be substantiated by adequate tests, subject to theapproval of the procuring or certificating regulatory agency. For edge margins between 1.5 and 2.0, linearinterpolation of properties may be used.Bearing design properties are applicable to t/D ratios from 0.25 to 0.50. Bearing design values forconditions of t/D < 0.25 or t/D > 0.50 must be substantiated by tests. The percentage curves showingtemperature effects on bearing stress may be used with both e/D properties of 1.5 and 2.0.Due to differences in results obtained between dry-pin and wet-pin tests, designers are encouraged toconsider the use of a reduction factor with published bearing stresses for use in design.1.4.8 TEMPERATURE EFFECTS — Temperature effects require additional considerations for static,fatigue and fracture toughness properties. In addition, this subject introduces concerns for time-dependentcreep properties.18.104.22.168 Low Temperature — Temperatures below roomtemperature generally cause an increasein strength properties of metallic alloys. Ductility, fracture toughness, and elongation usually decrease. Forspecific information, see the applicable chapter and references noted therein.22.214.171.124 Elevated Temperature — Temperatures above room temperature usually cause adecrease in the strength properties of metallic alloys. This decrease is dependent on many factors, such astemperature and the time of exposure which may degrade the heat treatment condition, or cause a metallurgicalchange. Ductility may increase or decrease with increasing temperature depending on the same variables.Because of this dependence of strength and ductility at elevated temperatures on many variables, it isemphasized that the elevated temperature properties obtained from this Handbook be applied for only thoseconditions of exposure stated herein.The effect of temperature on static mechanical properties is shown by a series of graphs of property(as percentages of the room temperature allowable property) versus temperature. Data used to construct thesegraphs were obtained from tests conducted over a limited range of strain rates. Caution should be exercisedin using these static property curves at very high temperatures, particularly if the strain rate intended in designis much less than that stated with the graphs. The reason for this concern is that at very low strain rates orunder sustained loads, plastic deformation or creep deformation may occur to the detriment of the intendedstructural use.
MIL-HDBK-5H, Change Notice 11 October 20011-11Supersedes Chapter 1 of Revision HFigure 126.96.36.199.2. Typical creep-rupture curve.188.8.131.52.1 Creep and Stress-Rupture Properties — Creep is defined as a time-dependentdeformation of a material while under an applied load. It is usually regarded as an elevated temperaturephenomenon, although some materials creep at room temperature. If permitted to continue indefinitely, creepterminates in rupture. Since creep in service is usually typified by complex conditions of loading andtemperature, the number of possible stress-temperature-time profiles is infinite. For economic reasons, creepdata for general design use are usually obtained under conditions of constant uniaxial loading and constanttemperature in accordance with Reference 184.108.40.206.1(a). Creep data are sometimes obtained under conditionsof cyclic uniaxial loading and constant temperature, or constant uniaxial loading and variable temperatures.Section 9.3.6 provides a limited amount of creep data analysis procedures. It is recognized that, whensignificant creep appears likely to occur, it maybe necessary to test under simulated service conditions becauseof difficulties posed in attempting to extrapolate from simple to complex stress-temperature-time conditions.Creep damage is cumulative similar to plastic strain resulting from multiple static loadings. Thisdamage may involve significant effects on the temper of heat treated materials, including annealing, and theinitiation and growth of cracks or subsurface voids within a material. Such effects are often recognized asreductions in short time strength properties or ductility, or both.220.127.116.11.2 Creep-Rupture Curve — Results of tests conducted under constant loading and constanttemperature are usually plotted as strain versus time up to rupture. A typical plot of this nature is shown inFigure 18.104.22.168.2. Strain includes both the instantaneous deformation due to load application and the plasticstrain due to creep. Other definitions and terminology are provided in Section 22.214.171.124.126.96.36.199.3 Creep or Stress-Rupture Presentations — Results of creep or stress-rupture testsconducted over a range of stresses and temperatures are presented as curves of stress versus the logarithm oftime to rupture. Each curve represents an average, best-fit description of measured behavior. Modificationof such curves into design use are the responsibility of the design community since material applications andregulatory requirements may differ. Refer to Section 9.3.6 for data reduction and presentation methods andReferences 188.8.131.52.1(b) and (c).
MIL-HDBK-5H, Change Notice 11 October 20011-12Supersedes Chapter 1 of Revision H1.4.9 FATIGUE PROPERTIES — Repeated loads are one of the major considerations for design of bothcommercial and military aircraft structures. Static loading, preceded by cyclic loads of lesser magnitudes, mayresult in mechanical behaviors (Ftu , Fty , etc.) lower than those published in room temperature allowablestables. Such reductions are functions of the material and cyclic loading conditions. A fatigue allowablesdevelopment philosophy is not presented in this Handbook. However, basic laboratory test data are useful formaterials selection. Such data are therefore provided in the appropriate materials sections.In the past, common methods of obtaining and reporting fatigue data included results obtained fromaxial loading tests, plate bending tests, rotating bending tests, and torsion tests. Rotating bending tests applycompletely reversed (tension-compression) stresses to round cross section specimens. Tests of this type arenow seldom conducted for aerospace use and have therefore been dropped from importance in this Handbook.For similar reasons, flexural fatigue data also have been dropped. No significant amount of torsional fatiguedata have ever been made available. Axial loading tests, the only type retained in this Handbook, consist ofcompletelyreversed loadingconditions (mean stress equals zero) and those in which the mean stresswas variedto create different stress (or strain) ratios (R = minimum stress or strain divided by maximum stress or strain).Refer to Reference 1.4.9(a) for load control fatigue testing guidelines and Reference 1.4.9(b) for strain controlfatigue testing guidelines.184.108.40.206 Terminology — A number of symbols and definitions are commonly used to describefatigue test conditions, test results and data analysis techniques. The most important of these are described inSection 220.127.116.11.18.104.22.168 Graphical Display of Fatigue Data — Results of axial fatigue tests are reported onS-N and ε - N diagrams. Figure 22.214.171.124(a) shows a family of axial load S-N curves. Data for each curverepresents a separate R-value.S-N and ε - N diagrams are shown in this Handbook with the raw test data plotted for each stress orstrain ratio or, in some cases, for a single value of mean stress. A best-fit curve is drawn through the data ateach condition. Rationale used to develop best-fit curves and the characterization of all such curves in a singlediagram is explained in Section 9.3.4. For load control test data, individual curves are usually based on anequivalent stress which consolidates data for all stress ratios into a single curve. Refer to Figure 126.96.36.199(b).For strain control test data, an equivalent strain consolidation method is used.Elevated temperature fatigue test data are treated in the same manner as roomtemperature data, as longas creep is not a significant factor and room temperature analysis methods can be applied. In the limitednumber of cases where creep strain data have been recorded as a part of an elevated temperature fatigue testseries, S-N (or ε - N) plots are constructed for specific creep strain levels. This is provided in addition to thecustomary plot of maximum stress (or strain) versus cycles to failure.The above information may not apply directly to the design of structures for several reasons. First,Handbook information may not take into account specific stress concentrations unique to any given structuraldesign. Designconsiderationsusuallyincludestressconcentrationscausedbyreentrantcorners,notches,holes,joints, rough surfaces, structural damage, and other conditions. Localized high stresses induced during thefabrication of some parts have a much greater influence on fatigue properties than on static properties.These factors significantly reduce fatigue life below that which is predictable by estimating smooth specimenfatigue performance with estimated stresses due to fabrication. Fabricated parts have been found to fail at lessthan 50,000 cycles of loading when the nominal stress was far below that which could be repeated manymillions of times using a smooth machined test specimen.
MIL-HDBK-5H, Change Notice 11 October 20011-13Supersedes Chapter 1 of Revision HFatigue Life, Cycles103 104 105 106 107 108MaximumStress,ksi01020304050607080+ ++ ++ +++ ++ + + ++ +++ + +++ +++++ +++++++xxxxxxxxxxxxx xx→→→→→→→→→→→→→→→..on net section.Note: Stresses are basedMean Stress or Stress Ratio =Level 2Level 1Level 4xLevel 3+Material=A, Kt=B, Notch Type=C,Runout→Figure 188.8.131.52(a). Best fit S/N curve diagram for a material at various stress ratios.Fatigue Life, Cycles103 104 105 106 107 108EquivalentStress,Seq0102030405060708090100+ ++ ++ +++ ++ ++++ +++ + +++ ++++++xxxxxxxxxxxxx..on net section.Note: Stresses are basedMean Stress or Stress Ratio =Level 2Level 1Level 4xLevel 3+Material=A, Kt=B, Notch Type=C,Figure 184.108.40.206(b). Consolidated fatigue data for a material using the equivalentstress parameter.
MIL-HDBK-5H, Change Notice 11 October 20011-14Supersedes Chapter 1 of Revision HNotchedfatiguespecimentestdataareshowninvariousHandbookfigurestoprovideanunderstandingof deleterious effects relative to results for smooth specimens. All of the mean fatigue curves published in thisHandbook, including both the notched fatigue and smooth specimen fatigue curves, require modification intoallowables for design use. Such factors may impose a penalty on cyclic life or upon stress. This is aresponsibility for the design community. Specific reductions vary between users of such information, anddepend on the criticality of application, sources of uncertainty in the analysis, and requirements of thecertificating activity. References 220.127.116.11(a) and (b) contain more specific information on fatigue testingprocedures, organization of test results, influences of various factors, and design considerations.1.4.10 METALLURGICAL INSTABILITY — In addition to the retention of strength and ductility, astructural material must also retain surface and internal stability. Surface stability refers to the resistance ofthe material to oxidizing or corrosive environments. Lack of internal stability is generally manifested (in someferrous and several other alloys) by carbide precipitation, spheroidization, sigma-phase formation, temperembrittlement, and internal or structural transformation, depending upon the specific conditions of exposure.Environmental conditions, which influence metallurgical stability include heat, level of stress,oxidizing or corrosive media and nuclear radiation. The effect of environment on the material can be observedas either improvement or deterioration of properties, depending upon the specific imposed conditions. Forexample, prolonged heating may progressively raise the strength of a metallic alloy as measured on smoothtensile or fatigue specimens. However, at the same time, ductility may be reduced to such an extent thatnotched tensile or fatigue behavior becomes erratic or unpredictable. The metallurgy of each alloy should beconsidered in making material selections.Under normal temperatures, i.e., between -65EF and 160EF, the stability of most structural metallicalloys is relatively independent of exposure time. However, as temperature is increased, the metallurgicalinstability becomes increasingly time dependent. The factor of exposure time should be considered in designwhen applicable.1.4.11 BIAXIAL PROPERTIES — Discussions up to this point pertained to uniaxial conditions of static,fatigue and creep loading. Many structural applications involve both biaxial and triaxial loadings. Becauseof the difficulties of testing under triaxial loading conditions, few data exist. However, considerable biaxialtesting has been conducted and the following paragraphs describe how these results are presented in thisHandbook. This does not conflict with data analysis methods presented in Chapter 9. Therein, statisticalanalysis methodology is presented solely for use in analyzing test data to establish allowables.If stress axes are defined as being mutually perpendicular along x-, y-, and z-directions in a rectangularcoordinate system, a biaxial stress is then defined as a condition in which loads are applied in both of the x-and y-directions. In some special cases, loading may be applied in the z-direction instead of the y-direction.Most of the following discussion will be limited to tensile loadings in the x- and y-directions. Stresses andstrains in these directions are referred to as principal stresses and principal strains. See Reference 1.4.11.When a specimen is tested under biaxial loading conditions, it is customary to plot the results as abiaxial stress-strain diagram. These diagrams are similar to uniaxial stress-strain diagrams shown in Figure1.4.4. Usually, only the maximum (algebraically larger) principal stress and strain are shown for each testresult. When tests of the same material are conducted at different biaxial stress ratios, the resulting curves maybe plotted simultaneously, producing a family of biaxial stress-strain curves as shown in Figure 1.4.11 for anisotropic material. For anisotropic materials, biaxial stress-strain curves also require distinction by graindirection.
MIL-HDBK-5H, Change Notice 11 October 20011-15Supersedes Chapter 1 of Revision HFigure 1.4.11. Typical biaxial stress-strain diagramsfor isotropic materials.The reference direction for a biaxial stress ratio, i.e., the direction corresponding to B=0, should beclearly indicated with each result. The reference direction is always considered as the longitudinal (rolling)direction for flat products and the hoop (circumferential) direction for shells of revolution, e.g., tubes, cones,etc. The letter B denotes the ratio of applied stresses in the two loading directions. For example, B-values of2, 0.5 shown in Figure 1.4.11 indicate results representing both biaxial stress ratios of 2 or 0.5, since this isa hypothetical example for an isotropic material, e.g., cross-rolled sheet. In a similar manner, the curve labeledB=1 indicates a biaxial stress-strain result for equally applied stresses in both directions. The curve labeledB = 4, 0 indicates the biaxial stress-strain behavior when loading is applied in only one direction, e.g., uniaxialbehavior. Biaxial property data presented in the Handbook are to be considered as basic material propertiesobtained from carefully prepared specimens.18.104.22.168 Biaxial Modulus of Elasticity— Referringto Figure 1.4.11, it is noted that the originalportion of each stress-strain curve is essentially a straight line. In uniaxial tension or compression, the slopeof this line is defined as the modulus of elasticity. Under biaxial loading conditions, the initial slope of suchcurves is defined as the biaxial modulus. It is a function of biaxial stress ratio and Poisson’s ratio. SeeEquation 22.214.171.124.126.96.36.199 Biaxial Yield Stress — Biaxial yield stress is defined as the maximum principal stresscorresponding to 0.002 in./in. plastic strain in the same direction, as determined from a test curve.In the design of aerospace structures, biaxial stress ratios other than those normally used in biaxialtesting are frequently encountered. Information can be combined into a single diagramto enable interpolationsat intermediate biaxial stress ratios, as shown in Figure 188.8.131.52. An envelope is constructed through testresults for each tested condition of biaxial stress ratios. In this case, a typical biaxial yield stress envelope isidentified. In the preparation of such envelopes, data are first reduced to nondimensional form (percent ofuniaxial tensile yield stress in the specified reference direction), then a best-fit curve is fitted through thenondimensionalized data. Biaxial yield strength allowables are then obtained by multiplying the uniaxial Fty(or Fcy) allowable by the applicable coordinate of the biaxial stress ratio curve. To avoid possible confusion,the reference direction used for the uniaxial yield strength is indicated on each figure.
MIL-HDBK-5H, Change Notice 11 October 20011-16Supersedes Chapter 1 of Revision HFigure 184.108.40.206. Typical biaxial yield stressenvelope.220.127.116.11 Biaxial Ultimate Stress — Biaxial ultimate stress is defined as the highest nominalprincipal stress attained in specimens of a given configuration, tested at a given biaxial stress ratio. Thisproperty is highly dependent upon geometric configuration of the test parts. Therefore, such data should belimited in use to the same design configurations.The method of presenting biaxial ultimate strength data is similar to that described in the precedingsection for biaxial yield strength. Both biaxial ultimate strength and corresponding uniform elongation dataare reported, when available, as a function of biaxial stress ratio test conditions.1.4.12 FRACTURE TOUGHNESS — The occurrence of flaws in a structural component is anunavoidable circumstance of material processing, fabrication, or service. Flaws may appear as cracks, voids,metallurgical inclusions, weld defects, design discontinuities, or some combination thereof. The fracturetoughness of a part containing a flaw is dependent upon flaw size, component geometry, and a materialproperty defined as fracture toughness. The fracture toughness of a material is literally a measure of itsresistance to fracture. As with other mechanical properties, fracture toughness is dependent upon alloy type,processing variables, product form, geometry, temperature, loading rate, and other environmental factors.This discussion is limited to brittle fracture, which is characteristic of high strength materials underconditions of loading resulting in plane-strain through the cross section. Very thin materials are described asbeing under the condition of plane-stress. The following descriptions of fracture toughness properties appliesto the currently recognized practice of testing specimens under slowly increasing loads. Attendant andinteracting conditions of cyclic loading, prolonged static loadings, environmental influences other thantemperature, and high strain rate loading are not considered.18.104.22.168 Brittle Fracture — For materials that have little capacity for plastic flow, or for flaw andstructural configurations, which induce triaxial tension stress states adjacent to the flaw, component behavioris essentially elastic until the fracture stress is reached. Then, a crack propagates from the flaw suddenly andcompletely through the component. A convenient illustration of brittle fracture is a typical load-compliancerecord of a brittle structural component containing a flaw, as illustrated in Figure 22.214.171.124. Since little or noplastic effects are noted, this mode is termed brittle fracture.
MIL-HDBK-5H, Change Notice 11 October 20011-17Supersedes Chapter 1 of Revision HFigure 126.96.36.199. Typical load-deformation recordof a structural component containing a flawsubject to brittle fracture.This mode of fracture is characteristic of the very high-strength metallic materials under plane-strainconditions.188.8.131.52 Brittle Fracture Analysis — The application of linear elastic fracture mechanics hasled to the stress intensity concept to relate flaw size, component geometry, and fracture toughness. In its verygeneral form, the stress intensity factor, K, can be expressed as[184.108.40.206]K f aY ksi in= ⋅, . /1 2wheref = stress applied to the gross, flaws section, ksia = measure of flaw size, inchesY = factor relating component geometry and flaw size, nondimensional. SeeReference 220.127.116.11(a) for values.For every structural material, which exhibits brittle fracture (by nature of low ductility or plane-strainstress conditions), there is a lower limiting value of K termed the plane-strain fracture toughness, KIc.Thespecificapplicationofthisrelationshipisdependentonflawtype,structuralconfigurationandtypeof loading, and a variety of these parameters can interact in a real structure. Flaws may occur through thethickness, may be imbedded as voids or metallurgical inclusions, or may be partial-through (surface) cracks.Loadings of concern may be tension and/or flexure. Structural components may vary in section size and maybe reinforced in some manner. The ASTM Committee E 8 on Fatigue and Fracture has developed testing andanalytical techniques for many practical situations of flaw occurrence subject to brittle fracture. They aresummarized in Reference 18.104.22.168(a).
MIL-HDBK-5H, Change Notice 11 October 20011-18Supersedes Chapter 1 of Revision HFigure 22.214.171.124. Typical principal fracture pathdirections.126.96.36.199 Critical Plane-Strain Fracture Toughness — A tabulation of fracture toughnessdata is printed in the general discussion prefacing most alloy chapters in this Handbook. These critical plane-strain fracture toughness values have been determined in accordance with recommended ASTM testingpractices. This information is provided for information purposes only due to limitations in available dataquantities and product form coverages. The statistical reliability of these properties is not known. Listedproperties generally represent the average value of a series of test results.Fracture toughness of a material commonly varies with grain direction. When identifying either testresults or a general critical plane strain fracture toughness average value, it is customary to specify specimenand crack orientations by an ordered pair of grain direction symbols. The first digit denotes the grain directionnormal to the crack plane. The second digit denotes the grain direction parallel to the fracture plane. For flatsections of various products, e.g., plate, extrusions, forgings, etc., in which the three grain directions aredesignated (L) longitudinal, (T) transverse, and (S) short transverse, the six principal fracture path directionsare: L-T, L-S, T-L, T-S, S-L and S-T. Figure 188.8.131.52 identifies these orientations.184.108.40.206.1 Environmental Effects — Cyclic loading, even well below the fracture threshold stress,may result in the propagation of flaws, leading to fracture. Strain rates in excess of standard static rates maycause variations in fracture toughness properties. There are significant influences of temperature on fracturetoughness properties. Temperature effects data are limited. These information are included in each alloysection, when available.Under the condition of sustained loading, it has been observed that certain materials exhibit increasedflaw propagation tendencies when situated in either aqueous or corrosive environments. When such is knownto be the case, appropriate precautionary notes have been included with the standard fracture toughnessinformation.220.127.116.11 Fracture in Plane-Stress and Transitional-Stress States — Plane-strainconditions do not describe the condition of certain structural configurations which are either relatively thin orexhibit appreciable ductility. In these cases, the actual stress state may approach the opposite extreme, plane-
MIL-HDBK-5H, Change Notice 11 October 20011-19Supersedes Chapter 1 of Revision HFigure 18.104.22.168. Typical load-deformationrecord for non-plane strain fracture.stress, or, more generally, some intermediate- or transitional-stress state. The behavior of flaws and cracksunder these conditions is different from those of plane-strain. Specifically, under these conditions, significantplastic zones can develop ahead of the crack or flaw tip, and stable extension of the discontinuity occurs as aslow tearing process. This behavior is illustrated in a compliance record by a significant nonlinearity prior tofracture as shown in Figure 22.214.171.124. This nonlinearity results from the alleviation of stress at the crack tip bycausing plastic deformation.126.96.36.199.1 Analysis of Plane-Stress and Transitional-Stress State Fracture — The basicconcepts of linear elastic fracture mechanics as used in plane-strain fracture analysis also applies to theseconditions. The stress intensity factor concept, as expressed in general form by Equation 188.8.131.52, is used torelate load or stress, flaw size, component geometry, and fracture toughness.However, interpretation of the critical flaw dimension and corresponding stress has two possibilities.This is illustrated in Figure 184.108.40.206.1. One possibility is the onset of nonlinear displacement with increasingload. The other possibility identifies the fracture condition, usually very close to the maximum load.Generally, these two conditions are separated in applied stress and exhibit large differences in flaw dimensionsdue to stable tearing.When a compliance record is transformed into a crack growth curve, the difference between the twopossible K-factor designations becomes more apparent. In most practical cases, the definition of nonlinearcrack length with increasing load is difficult to assess. As a result, an alternate characterization of this behavioris provided by defining an artificial or “apparent” stress intensity factor.[220.127.116.11.1]K f a Yapp o=
MIL-HDBK-5H, Change Notice 11 October 20011-20Supersedes Chapter 1 of Revision HFigure 18.104.22.168.1. Crack growth curve.The apparent fracture toughness is computed as a function of the maximum stress and initial flaw size.This datum coordinate corresponds to point A in Figure 22.214.171.124.1. This conservative stress intensity factoris a first approximation to the actual property associated with the point of fracture.126.96.36.199 Apparent Fracture Toughness Values for Plane-Stress and Transitional-Stress States — When available, each alloy chapter contains graphical formats of stress versus flaw size.This is provided for each temper, product form, grain direction, thickness, and specimen configuration. Datapoints shown in these graphs represent the initial flaw size and maximum stress achieved. These data havebeen screened to assure that an elastic instability existed at fracture, consistent with specimen type. Theaverage Kapp curve, as defined in the following subsections, is shown for each set of data.188.8.131.52.1 Middle-Tension Panels — The calculation of apparent fracture toughness for middle-tension panels is given by the following equation.[184.108.40.206.1(a)]( )K f a a Wapp c o o= ⋅π πsec //1 2Data used to compute Kapp values have been screened to ensure that the net section stress at failure did notexceed 80 percent of the tensile yield strength; that is, they satisfied the criterion:[220.127.116.11.1(b)]f TYS a Wc ≤ −08 1 2. ( ) / ( / )This criterion assures that the fracture was an elastic instability and that plastic effects are negligible.The average Kapp parametric curve is presented on each figure as a solid line with multiple extensionswhere width effects are displayed in the data. As added information, where data are available, the propensityfor slow stable tearing prior to fracture is indicated by a crack extension ratio, ∆2a/2ao. The coefficient (2)indicates the total crack length; the half-crack length is designated by the letter “a.” In some cases, where dataexist covering a wide range of thicknesses, graphs of Kapp versus thickness are presented.1.4.13 FATIGUE CRACK GROWTH — Crack growth deals with material behavior between crackinitiation and crack instability. In small size specimens, crack initiation and specimen failure may be nearly
MIL-HDBK-5H, Change Notice 11 October 20011-21Supersedes Chapter 1 of Revision Hsynonymous. However, in larger structural components, the existence of a crack does not necessarily implyimminent failure. Significant structural life exists during cyclic loading and crack growth.18.104.22.168 Fatigue Crack Growth — Fatigue crack growth is manifested as the growth orextension of a crack under cyclic loading. This process is primarily controlled by the maximum load or stressratio. Additional factors include environment, loading frequency, temperature, and grain direction. Certainfactors, such as environment and loading frequency, have interactive effects. Environment is important froma potential corrosion viewpoint. Time at stress is another important factor. Standard testing procedures aredocumented in Reference 22.214.171.124.Fatigue crack growth data presented herein are based on constant amplitude tests. Crack growthbehaviors based on spectrum loading cycles are beyond the scope of this Handbook. Constant amplitude dataconsist of cracklength measurements at correspondingloadingcycles. Such data are presented ascrackgrowthcurves as shown in Figure 126.96.36.199(a).Since the crack growth curve is dependent on initial crack length and the loading conditions, the aboveformat is not the most efficient form to present information. The instantaneous slope, ∆a/∆N, correspondingto a prescribed number of loading cycles, provides a more fundamental characterization of this behavior. Ingeneral, fatigue crack growth rate behavior is evaluated as a function of the applied stress intensity factorrange, ∆K, as shown in Figure 188.8.131.52(b).184.108.40.206 Fatigue Crack Growth Analysis — It is known that fatigue-crack-growth behaviorunder constant-amplitude cyclic conditions is influenced by maximum cyclic stress, Smax, and some measureof cyclic stress range, ∆S (such as stress ratio, R, or minimum cyclic stress, Smin), the instantaneous crack size,a,andotherfactorssuchasenvironment,frequency,andtemperature. Thus,fatigue-crack-growthratebehaviorcan be characterized, in general form, by the relationda/dN . ∆a/∆N = g(Smax, ∆S or R or Smin, a, ...). [220.127.116.11(a)]By applying concepts of linear elastic fracture mechanics, the stress and crack size parameters can becombined into the stress-intensity factor parameter, K, such that Equation 18.104.22.168(a) may be simplified toda/dN . ∆a/∆N = g(Kmax, ∆K, ...) [22.214.171.124(b)]whereKmax = the maximum cyclic stress-intensity factor∆K = (1-R)Kmax, the range of the cyclic stress-intensity factor, for R $ 0∆K = Kmax, for R # 0.At present, in the Handbook, the independent variable is considered to be simply ∆K and the data are con-sidered to be parametric on the stress ratio, R, such that Equation 126.96.36.199(b) becomesda/dN . ∆a/∆N = g(∆K, R). [188.8.131.52(c)]184.108.40.206 Fatigue Crack Growth Data Presentation — Fatigue crack growth rate data forconstant amplitude cyclic loading conditions are presented as logarithmic plots of da/dN versus ∆K. Suchinformation, such as that illustrated in Figure 220.127.116.11, are arranged by material alloy and heat treatmentcondition. Each curve represents a specific stress ratio, R, environment, and cyclic loadingfrequency. Specificdetails regarding test procedures and data interpolations are presented in Chapter 9.
MIL-HDBK-5H, Change Notice 11 October 20011-22Supersedes Chapter 1 of Revision HFigure 18.104.22.168(a). Fatigue crack-growthcurve.Figure 22.214.171.124(b). Fatigue crack-growth-ratecurve.
MIL-HDBK-5H, Change Notice 11 October 20011-23Supersedes Chapter 1 of Revision HFigure 126.96.36.199. Sample display of fatigue crack growth rate data.
MIL-HDBK-5H, Change Notice 11 October 20011-24Supersedes Chapter 1 of Revision H1.5 TYPES OF FAILURES1.5.1 GENERAL — In the following discussion, failure will usually indicate fracture of a member orthe condition of a member when it has attained maximum load.1.5.2 MATERIAL FAILURES — Fracture can occur in either ductile or brittle fashions in the samematerial depending on the state of stress, rate of loading, and environment. The ductility of a material has asignificant effect on the ability of a part to withstand loading and delay fracture. Although not a specific designproperty for ductile materials, some ductility data are provided in the Handbook to assist in material selections.The following paragraphs discuss the relationship between failure and the applied or induced stresses.188.8.131.52 Direct Tension or Compression — This type of failureis associated with ultimatetensile or compressive stress of the material. For compression, it can only apply to members having large crosssectional dimensions relative to their lengths. See Section 184.108.40.206.220.127.116.11 Shear — Pure shear failures are usually obtained when the shear load is transmitted overa very short length of a member. This condition is approached in the case of rivets and bolts. In cases whereultimate shear stress is relatively low, a pure shear failure can result. But, generally members subjected toshear loads fail under the action of the resulting normal stress, usually the compressive stress. See Equation18.104.22.168. Failure of tubes in torsion are not caused by exceeding the shear ultimate stress, but by exceeding anormal compressive stress which causes the tube to buckle. It is customary to determine stresses for memberssubjected to shear in the form of shear stresses although they are actually indirect measures of the stressesactually causing failure.22.214.171.124 Bearing — Failure of a material in bearing can consist of crushing, splitting, tearing, orprogressive rapid yielding in the direction of load application. Failure of this type depends on the relative sizeand shape of the two connecting parts. The maximum bearing stress may not be applicable to cases in whichone of the connecting members is relatively thin.126.96.36.199 Bending — For sections not subject to geometric instability, a bending failure can beclassed as either a tensile or compressive failure. Reference 188.8.131.52 provides methodology by which actualbending stresses above the material proportional limit can be used to establish maximum stress conditions.Actual bending stresses are related to the bending modulus of rupture. The bending modulus of rupture (fb)is determined by Equation 184.108.40.206. When the computed bending modulus of rupture is found to be lower thanthe proportional limit strength, it represents an actual stress. Otherwise, it represents an apparent stress, andis not considered as an actual material strength. This is important when considering complex stress states, suchas combined bending and compression or tension.220.127.116.11 Failure Due to Stress Concentrations — Static stress properties represent pristinematerials without notches, holes, or other stress concentrations. Such simplistic structural design is not alwayspossible. Consideration should be given to the effect of stress concentrations. When available, references arecited for specific data in various chapters of the Handbook.18.104.22.168 Failure from Combined Stresses — Under combined stress conditions, where failureis not due to buckling or instability, it is necessary to refer to some theory of failure. The “maximum shear”theory is widely accepted as a working basis in the case of isotropic ductile materials. It should be noted thatthis theory defines failure as the first yielding of a material. Any extension of this theory to cover conditionsof final rupture must be based on evidence supported by the user. The failure of brittle materials undercombined stresses is generally treated by the “maximum stress” theory. Section 1.4.11 contains a morecomplete discussion of biaxial behavior. References 22.214.171.124(a) through (c) offer additional information.
MIL-HDBK-5H, Change Notice 11 October 20011-25Supersedes Chapter 1 of Revision H1.5.3 INSTABILITY FAILURES — Practically all structural members, such as beams and columns,particularly those made from thin material, are subject to failure due to instability. In general, instability canbe classed as (1) primary or (2) local. For example, the failure of a tube loaded in compression can occur eitherthrough lateral deflection of the tube acting as a column (primary instability) or by collapse of the tube wallsat stresses lower than those required to produce a general column failure. Similarly, an I-beam or other formedshape can fail by a general sidewise deflection of the compression flange, by local wrinkling of thinoutstanding flanges, or by torsional instability. It is necessary to consider all types of potential failures unlessit apparent that the critical load for one type is definitely the controlling condition.Instability failures can occur in either the elastic range below the proportional limit or in the plasticrange. These two conditions are distinguished by referring to either “elastic instability” or “plastic instability”failures. Neither type of failure is associated with a material’s ultimate strength, but largely depends upongeometry.A method for determining the local stability of aluminum alloy column sections is provided inReference 1.7.1(b). Documents cited therein are the same as those listed in References 126.96.36.199(a) through (e).188.8.131.52 Instability Failures Under Compression — Failures of this type are discussed inSection 1.6 (Columns).184.108.40.206 Instability Failures Under Bending — Round tubes when subjected to bending aresubject to plastic instability failures. In such cases, the failure criterion is the modulus of rupture. Equation220.127.116.11, which was derived from theory and confirmed empirically with test data, is applicable. Elasticinstability failures of thin walled tubes having high D/t ratios are treated in later sections.18.104.22.168 Instability Failures Under Torsion — The remarks given in the preceding sectionapply in a similar manner to round tubes under torsional loading. In such cases, the modulus of rupture intorsion is derived through the use of Equation 22.214.171.124. See Reference 126.96.36.199.188.8.131.52 Failure Under Combined Loadings — For combined loading conditions in whichfailure is caused by buckling or instability, no theory exists for general application. Due to the various designphilosophies and analytical techniques used throughout the aerospace industry, methods for computing marginof safety are not within the scope of this Handbook.1.6 COLUMNS1.6.1 GENERAL — A theoretical treatment of columns can be found in standard texts on the strengthof materials. Some of the problems which are not well defined by theory are discussed in this section. Actualstrengths of columns of various materials are provided in subsequent chapters.1.6.2 PRIMARY INSTABILITY FAILURES — A column can fail through primary instability by bendinglaterally (stable sections) or by twisting about some axis parallel to its own axis. This latter type of primaryfailure is particularly common to columns having unsymmetrical open sections. The twisting failure of aclosed section column is precluded by its inherently high torsional rigidity. Since the amount of availableinformation is limited, it is advisable to conduct tests on all columns subject to this type of failure.184.108.40.206 Columns with Stable Sections — The Euler formula for columns which fail by lateralbending is given by Equation 220.127.116.11. A conservative approach in using this equation is to replace the elasticmodulus (E) by the tangent modulus (Et) given by Equation 18.104.22.168. Values for the restraint coefficient (c)depend on degrees of ends and lateral fixities. End fixities tend to modify the effective column length as
MIL-HDBK-5H, Change Notice 11 October 20011-26Supersedes Chapter 1 of Revision Hindicated in Equation 22.214.171.124. For a pin-ended column having no end restraint, c = 1.0 and LN = L. A fixitycoefficient of c = 2 corresponds to an effective column length of LN = 0.707 times the total length.The tangent modulus equation takes into account plasticity of a material and is valid when thefollowing conditions are met:(a) The column adjusts itself to forcible shortening only by bending and not by twisting.(b) No buckling of any portion of the cross section occurs.(c) Loading is applied concentrically along the longitudinal axis of the column.(d) The cross section of the column is constant along its entire length.MIL-HDBK-5 provides typical stress versus tangent modulus diagrams for manymaterials, forms, andgrain directions. These information are not intended for design purposes. Methodologyis contained in Chapter9 for the development of allowable tangent modulus curves.126.96.36.199 Column Stress (fco) — The upper limit of column stress for primary failure is designatedas fco. By definition, this termshould not exceed the compression ultimate strength, regardless of how the latterterm is defined.188.8.131.52 Other Considerations — Methods of analysis by which column failure stresses can becomputed, accounting for fixities, torsional instability, load eccentricity, combined lateral loads, or varyingcolumn sections are contained in References 184.108.40.206(a) through (d).1.6.3 LOCAL INSTABILITY FAILURES — Columns are subject to failure by local collapse of walls atstresses below the primary failure strength. The buckling analysis of a column subject to local instabilityrequires consideration of the shape of the column cross section and can be quite complex. Local buckling,which can combine with primary buckling, leads to an instability failure commonly identified as crippling.220.127.116.11 Crushing or Crippling Stress (fcc) — The upper limit of column stress for local failureis defined by either its crushing or crippling stress. The strengths of round tubes have been thoroughlyinvestigated and considerable amounts of test results are available throughout literature. Fewer data areavailable for other cross sectional configurations and testingis suggested to establish specific information, e.g.,the curve of transition from local to primary failure.1.6.4 CORRECTION OF COLUMN TEST RESULTS — In the case of columns having unconventionalcross sections which are subject to local instability, it is necessary to establish curves of transition from localto primary failure. In determining these column curves, sufficient tests should be made to cover the followingpoints.18.104.22.168 Nature of “Short Column Curve” — Test specimens should cover a range of LN/ρvalues. When columns are to be attached eccentrically in structural application, tests should be designed tocover such conditions. This is important particularly in the case of open sections, as maximum load carryingcapabilities are affected by locations of load and reaction points.22.214.171.124 Local Failure — When local failure occurs, the crushing or crippling stress can bedetermined by extending the short column curve to a point corresponding to a zero value for LN/ρ. When afamily of columns of the same general cross section is used, it is often possible to determine a relationshipbetween crushing or crippling stress and some geometric factor. Examples are wall thickness, width, diameter,or some combination of these dimensions. Extrapolation of such data to conditions beyond test geometryextremes should be avoided.
MIL-HDBK-5H, Change Notice 11 October 20011-27Supersedes Chapter 1 of Revision H126.96.36.199 Reduction of Column Test Results on Aluminum and Magnesium Alloys toStandard Material — The use of correction factors provided in Figures 188.8.131.52(a) through (i) is acceptableto the Air Force, the Navy, the Army, and the Federal Aviation Administration for use in reducing aluminumand magnesium alloys column test data into allowables. (Note that an alternate method is provided in Section184.108.40.206). In using Figures 220.127.116.11(a) through (i), the correction of column test results to standard material ismade by multiplying the stress obtained from testing a column specimen by the factor K. This factor may beconsidered applicable regardless of the type of failure involved, i.e., column crushing, crippling or twisting.Note that not all the information provided in these figures pertains to allowable stresses, as explained below.The following terms are used in reducing column test results into allowable column stress:Fcy is the design compression yield stress of the material in question, applicable to the gage, temper andgrain direction along the longitudinal axis of a test column.FcN is the maximum test column stress achieved in test. Note that a letter (F) is used rather the customarylower case (f). This value can be an individual test result.FcyN is the compressive yield strength of the column material. Note that a letter (F) is used rather than thecustomary lower case (f). This value can be an individual test result using a standard compression testspecimen.Using the ratio of (FcN / FcyN), enter the appropriate diagram along the abscissa and extend a line upwards to theintersection of a curve with a value of (FcyN / FcyN). Linear interpolation between curves is permissible. At thislocation, extend a horizontal line to the ordinate and read the corresponding K-factor. This factor is then usedas a multiplier on the measured column strength to obtain the allowable. The basis for this allowable is thesame as that noted for the compression yield stress allowable obtained from the room temperature allowablestable.If the above method is not feasible, due to an inability of conducting a standard compression test ofthe column material, the compression yield stress of the column material may be estimated as follows: Conducta standard tensile test of the column material and obtain its tensile yield stress. Multiply this value by the ratioof compression-to-tensile yield allowables for the standard material. This provides the estimated compressionyield stress of the column material. Continue with the analysis as described above using the compression stressof a test column in the same manner.If neither of the above methods are feasible, it may be assumed that the compressive yield stressallowable for the column is 15 percent greater than minimum established allowable longitudinal tensile yieldstress for the material in question.18.104.22.168 Reduction of Column Test Results to Standard Material--Alternate Method— For materials that are not covered by Figures 22.214.171.124(a) through (i), the following method is acceptable forall materials to the Air Force, the Navy, the Army, and the Federal Aviation Administration.(1) Obtain the column material compression properties: Fcy, Ec, nc.(2) Determine the test material column stress (fcN) from one or more column tests.(3) Determine the test material compression yield stress (fcyN) from one or more tests.(4) Assume Ec and nc from (1) apply directly to the column material. They should be the same material.
MIL-HDBK-5H, Change Notice 11 October 20011-28Supersedes Chapter 1 of Revision H=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.=Compressive yield stress (std)Column material compressive yield stressFcyFcyFcy.90.951.001.051.101.126.96.36.1991.35FcyFcyFcFigure 188.8.131.52(a). Nondimensional material correction chartfor 2024-T3 sheet.Fc=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.90.951.001.051.101.184.108.40.2061.35Figure 220.127.116.11(b). Nondimensional material correction chartfor 2024-T3 clad sheet.
MIL-HDBK-5H, Change Notice 11 October 20011-29Supersedes Chapter 1 of Revision HFc=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.90.951.001.051.101.18.104.22.1681.35Figure 22.214.171.124(c). Nondimensional material correction chartfor 2024-T4 extrusion less than 1/4 inch thick.Fc=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.90.951.001.051.101.126.96.36.1991.35Figure 188.8.131.52(d). Nondimensional material correction chartfor 2024-T4 extrusion 1/4 to 1-1/2 inches thick.
MIL-HDBK-5H, Change Notice 11 October 20011-30Supersedes Chapter 1 of Revision HFc=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.90.951.001.051.101.184.108.40.2061.35Figure 220.127.116.11(e). Nondimensional material correction chartfor 2024-T3 tubing.Fc=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.90.951.001.051.101.18.104.22.1681.35Figure 22.214.171.124(f). Nondimensional material correction chartfor clad 2024-T3 sheet.
MIL-HDBK-5H, Change Notice 11 October 20011-31Supersedes Chapter 1 of Revision HFc=Column material compressive yield stress0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.90.951.001.051.101.126.96.36.1991.35Figure 188.8.131.52(g). Nondimensional material correction chartfor 7075-T6 sheet.Fc=Column material compressive yield stress0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.901.001.101.201.30Figure 184.108.40.206(h). Nondimensional material correction chartfor AZ31B-F and AZ61A-F extrusion.
MIL-HDBK-5H, Change Notice 11 October 20011-32Supersedes Chapter 1 of Revision HFc=Column material compressive yield stress0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 1.1 1.2K=CorrectionFactor0.70.80.91.01.11.2Maximum test column Stress.Fcy=Compressive yield stress (std)Column material compressive yield stressFcyFcy FcyFcy.901.001.101.201.30Figure 220.127.116.11(i). Nondimensional material correction chartfor AZ31B-H24 sheet.(5) Assume that geometry of the test column is the same as that intended for design. This means that acritical slenderness ratio value of (LN/ρ) applies to both cases.(6) Using the conservative form of the basic column formula provided in Equation 18.104.22.168, this enablesan equality to be written between column test properties and allowables. If[22.214.171.124(a)]( ) ( )L for design L of thecolumn test/ /ρ ρ=Then[126.96.36.199(b)]( ) ( )Fc Et fordesign fc Et from test/ / =(7) Tangent modulus is defined as:[188.8.131.52(c)]E df det = /(8) Total strain (e) is defined as the sum of elastic and plastic strains, and throughout theHandbook is used as:[184.108.40.206(d)]e e eE p= +or,
MIL-HDBK-5H, Change Notice 11 October 20011-33Supersedes Chapter 1 of Revision H[220.127.116.11(e)]efEffyn= +0 002.So, Equation 18.104.22.168(c) can be rewritten as follows:[22.214.171.124(f)]EffEnfftyn=+0002.Tangent modulus, for the material in question, using its compression allowables is:[126.96.36.199(g)]EFFEnFFtccccccync=+0 002.In like manner, tangent modulus for the same material with the desired column configuration is:[188.8.131.52(h)]EffEnfftccccccync.=+0002Substitution of Equations 184.108.40.206(g) and 220.127.116.11(h) for their respective terms in Equation 18.104.22.168(b) andsimplifying provides the following relationship:[22.214.171.124(i)]FEnFFfEnffcccccyncccccync c+ = +0002 0002..The only unknown in the above equation is the term Fc , the allowable column compression stress. Thisproperty can be solved by an iterative process.This method is also applicable at other than room temperature, having made adjustments for the effectof temperature on each of the properties. It is critical that the test material be the same in all respectsas that for which allowables are selected from the Handbook. Otherwise, the assumption made inEquation 126.96.36.199(c) above is not valid. Equation 188.8.131.52(i) must account for such differences in moduliand shape factors when applicable.1.7 THIN-WALLED AND STIFFENED THIN-WALLED SECTIONSA bibliography of information on thin-walled and stiffened thin-walled sections is contained in References1.7(a) and (b).
MIL-HDBK-5H, Change Notice 11 October 20011-34Supersedes Chapter 1 of Revision HREFERENCES184.108.40.206 Goodman, S. and Russell, S.B., U.S. Air Force, “Poisson’s Ratio of Aircraft Sheet Materialsfor Large Strain,” WADC-TR-53-7, 58 pp (June1953).1.4.4 “Test Methods of Tension Testing of Metallic Materials,” ASTM E 220.127.116.11(a) Hyler, W.S., “An Evaluation of Compression-Testing Techniques for Determining ElevatedTemperature Properties of Titanium Sheet,” Titanium Metallurgical Laboratory Report No. 43,Battelle Memorial Institute, 38 pp, Appendix 28 pp (June 8, 1956).1.4.5(b) “Compression Testing of Metallic Materials at Room Temperature,” ASTM E 18.104.22.168 Stange, A.H., Ramberg, W. and Back, G., “Torsion Tests of Tubes,” National AdvisoryCommittee for Aeronautics, Report No. 601, pp 515-535 (Feb. 1937).1.4.7(a) Stickley, G.W. and Moore, A.A., “Effects of Lubrication and Pin Surface on Bearing Strengthsof Aluminum and Magnesium Alloys,” Materials Research and Standards, 2, (9), pp 747-751(September 1962).1.4.7(b) “Method of Pin-Type Bearing Test of Metallic Materials,” ASTM E 22.214.171.124.2.1(a) “Recommended Practice for Conducting Creep, Creep-Rupture, and Stress-Rupture Tests ofMetallic Materials,” ASTM E 126.96.36.199.2.1(b) Rice, Richard, “Reference Document for the Analysis of Creep and StressRupture Data in MIL-HDBK-5,” AFWAL-TR-81-4097 (September 1981).188.8.131.52.1(c) Aarnes, M.N. and Tuttle, M.M., “Presentation of Creep Data for Design Purposes,” ASDTechnical Report 61-216 (June 1961) (MCIC 45114).1.4.9(a) “Recommended Practice for Constant Amplitude Axial Fatigue Tests of Metallic Materials,”ASTM E 4184.108.40.206(b) “Recommended Practice for Constant-Amplitude Low-Cycle Fatigue Testing,” ASTM E 606.1.4.9.2(a) Grover, H.J., “Fatigue of Aircraft Structures,” Prepared for Naval Air Systems Command,Department of the Navy, 335 pp (1966).220.127.116.11(b) Osgood, C.C., “Fatigue Design,” Wiley-Interscience, A Division of John Wiley and Sons, Inc.,523 pp (1970).1.4.11 Bert, C.W., Mills, E.J. and Hyler, W.S., “Mechanical Properties of Aerospace Structural AlloysUnder Biaxial-Stress Conditions,” AFML-TR-66-229, (August 1966).18.104.22.168(a) “Standard Method of Test for Plane-Strain Fracture Toughness of Metallic Materials,” ASTME 322.214.171.124.1 “Test Method for Measurements of Fatigue Crack Growth Rates,” ASTM E 647.
MIL-HDBK-5H, Change Notice 11 October 20011-35Supersedes Chapter 1 of Revision H126.96.36.199 Paris, P.C., “The Fracture Mechanics Approach to Fatigue,” Proc. 10th Sagamore Conference,p. 107, Syracuse University Press (1965).188.8.131.52 Cozzone, F.P., “Bending Strength in the Plastic Range,” Journal of the Aeronautical Sciences,10, pp 137-151, (1943).184.108.40.206(a) Dieter, G.E., Jr., “Mechanical Metallurgy,” McGraw-Hill Book Company, Inc., 615 pp (1961).220.127.116.11(b) Freudenthal, A.M., “The Inelastic Behavior of Engineering Materials and Structures,” JohnWiley and Sons, Inc., New York, 587 pp (1950).18.104.22.168(c) Parker, E.R., “Brittle Behavior of Engineering Structures,” John Wiley and Sons, Inc., NewYork, 323 pp (1957).22.214.171.124 Lundquist, E.E., “Strength Tests of Thin-Walled Duralumin Cylinders in Pure Bending,” U.S.National Advisory Committee for Aeronautics, Technical Note No. 479, 17 pp (December1933).126.96.36.199(a) Hill, H.N. and Clark, J.W., “Straight-Line Column Formulas for AluminumAlloys,” AluminumCompany of America, Aluminum Research Laboratories, Technical Paper No. 12, 8 pp (1955).188.8.131.52(b) AFFDL-TR-69-42,“StressAnalysisManual,”AirForceFlightDynamicsLaboratory,AirForceSystems Command, Wright-Patterson Air Force Base (February 1970).184.108.40.206(c) “Astronautic Structure Manual,” George C. Marshall Space Flight Center (August 15, 1970).220.127.116.11(d) Niles, A.S., and Newell, J.S., “Airplane Structure,” 2, Third Edition, John Wiley and Sons(1943).1.7(a) “Index of Aircraft Structures Research Reports,” U.S. National Advisory Committee forAeronautics, Index No. 7E29, 40 pp (June 1947).1.7(b) Gerard, and Becker, H., “Handbook of Structural Stability,” National Advisory Committee forAeronautics Technical Note, Nos. 3781, 102 pp (July 1957); 3782, 72 pp (July 1957); 3783, 154pp (August 1957); 3784, 93 pp (August 1957); and 3785, 89 pp (August 1957).
MIL-HDBK-5H, Change Notice 11 October 20011-37Supersedes Chapter 1 of Revision HSPECIFICATIONS AND STANDARDS REQUISITIONForm ApprovedOMB No. 0704-0230Expires Dec 31, 1991Public reporting burden for this collection of information is estimated to average 30 minutes per response, including the time of reviewing instructions, searching existing data sources, gathering and maintainingthe data needed. And completing and reviewing the collection of information. Send comments regarding this burden estimate or any other aspect of this collection of information, including suggestions for reducingthis burden, to Washington Headquarters Services, Directorate for Information Operations and Reports, 1215 Jefferson Davis Highway, Suite 1204, Arlington, VA 22202-4302, and to the Office of Management andBudget, Paperwork Reduction Project (0704-0230), Washington, DC 20503. Please DO NOT RETURN your form to either of these addresses. Send your completed form to address in item 9 of instructions.1. CUSTOMER NUMBER (Mandatory for Repeat Orders to expedite requests), CAGE CODE, OR UIC NUMBER2. YOUR ADDRESS (Print or Type)! !G IF YOUR ADDRESS HAS CHANGED, X THISBLOCK! !3. ATTENTION:4. DOCUMENTS REQUESTEDa. STANDARDIZATION DOCUMENT NUMBERb. QUANTITY(Restricted to 5)c. TITLE(From DoD Index of Specifications and Standards)INSTRUCTIONS1. PRINT OR TYPE ALL INFORMATION.2. Enter your customer number, CAGE (formerly FSCM), or UICnumber at the top of this form. It will expedite your order.3. If you have a customer number, use the Telephone OrderEntry System (TOES) for telephone orders: (215) 697-1187between the hours of 8 a.m. and 8 p.m. Eastern StandardTime, Monday through Friday. See “Guide to PrivateIndustry” for details.4. Documents ordered must appear in the DoD Index ofSpecifications and Standards (DODISS) or DODISS Notice.Requests submitted on this form will speed service. Reorderforms will be enclosed with each shipment.5. Requests for Official Use Documents or documents withoutDistribution Statement “A” must be submitted via cognizantDoD Inspection Officer or Contract Administrator forcertification of “need to know.”6. Non Government Standardization Documents will not befurnished to commercial concerns. Copies may bepurchased from the appropriate Non GovernmentStandards Body.7. Questions concerning documents not listed in theDepartment of Defense Index of Specifications andStandards (DODISS) or DODISS Notice should be directedto: NPFC Attn: Code 105. Telephone: (215) 697-2667 or(215) 697-2179.8. Further information may be obtained from NPFC “Guideto Private Industry.” Order as GUIDE-1.9. FORWARD REQUEST TO:Standardization Document Order Desk700 Robbins AvenueBuilding #4, Section DPhiladelphia, PA 19111-50945. SIGNATURE OF REQUESTER 6. DATE SIGNED (YYMMDD) 7. CLOSING DATE (YYMMDD)(IFB, RFQ, or RFP)DD Form 1425, APR 90 Previous editions are obsolete 0102-LF-009